Optimization Design of MK-GGBS Based Geopolymer Repairing Mortar Based on Response Surface Methodology

There are several influencing factors in the preparation of MK (metakaolin)-GGBS (ground granulated blast furnace slag)-based geopolymer repair mortars, including the MK-GGBS ratio, the alkalinity of the alkali activator solution, the modulus of the alkali activator solution, and the water-to-solid ratio. There are interactions between these factors, such as the different alkaline and modulus requirements of MK and GGBS, the interaction between the alkaline and modulus of the alkali activator solution, and the influence of water throughout the process. The effect of these interactions on the geopolymer repair mortar is not fully understood, making optimization of the MK-GGBS repair mortar ratio difficult. Therefore, in this paper, the response surface methodology (RSM) was used to optimize the preparation of the repair mortar, with GGBS content, SiO2/Na2O molar ratio, Na2O/binder ratio, and water/binder ratio as influencing factors and 1 d compressive strength, 1 d flexural strength, and 1 d bond strength as evaluation indices. Additionally, the repair mortar’s overall performance was assessed in terms of setting time, long-term compressive and bond strength, shrinkage, water absorption, and efflorescence. The results show that RSM was successful in establishing a relationship between the repair mortar’s properties and the factors. The recommended values of the GGBS content, Na2O/binder ratio, SiO2/Na2O molar ratio, and water/binder ratio are 60%, 10.1%, 1.19, and 0.41, respectively. The optimized mortar meets the standard’s requirements for set time, water absorption, shrinkage values, and mechanical strength, with minimal visual efflorescence. The back-scattered electron (BSE) images and energy dispersive spectroscopy (EDS) analysis show that the geopolymer and cement have good interfacial adhesion, and a denser interfacial transition zone exists in the optimized proportion.


Introduction
The deterioration of concrete structures has piqued the interest of civil engineers worldwide [1][2][3]. New repair materials are constantly being developed to strengthen and repair deteriorated concrete structures. Geopolymer is a new environmentally friendly cementing material that can set and harden quickly with high early strength, good longterm performance, durability, and a low carbon footprint [4]. Geopolymers are thought to be able to replace Portland cement as new building cementing materials. In recent years, because the elastic modulus and Poisson's ratio of geopolymers are close to cement concrete [5,6] and it can bond well with cement concrete, people have gradually developed the application of geopolymer in concrete structural repair [7].
The original geopolymer repair materials were mostly based on MK, which possesses high late strength [8], good bonding capability [8,9], and good durability [10,11]. However, the necessity for high-temperature curing [12], poor early strength [8], poor flowability [13], and severe efflorescence substantially limit the use of MK-based polymers as repair materials [14]. Subsequent researchers found that the geopolymer could cure at room temperature, yielding a higher compressive strength by replacing MK with a specific 1 d flexural strength, and 1 d bond strength. Setting time, shrinkage, water absorption, efflorescence, and long-term compressive and bond strength tests were performed to evaluate the performance of the optimized mortar. The BSE and EDS were used to characterize the adhesion of the geopolymer to the cement interface. The findings of this paper will aid in further optimizing the mix ratio of MK-GGBS-based geopolymer repair mortar as well as understanding its comprehensive performance as a repair material.

Raw Materials
MK, GGBS, and ordinary Portland cement (OPC) used in this study are all commercially available materials. The chemical composition of the precursor was determined by X-ray fluorescence spectrometer (XRF), as shown in Table 1. MK has the same SiO 2 content as GGBS, but MK has more Al 2 O 3 and GGBS has more CaO. The microstructure of MK and GGBS is shown in Figure 1. MK is a flake and GGBS is an angular particle. Figure 2a and Table 2 show the particle size of the precursors, with the mean particle size (D50) of MK and GGBS being 4.5 µm and 13.17 µm, respectively. Figure 2b shows the XRD pattern of the precursor. The main crystalline phases of MK are corundum, pseudorutile, and zircon, while the main crystalline phases of GGBS are quartz and calcium magnesium phosphate. International Standards Organization (ISO) sand is used as fine aggregate, and its physical properties are shown in Table 3. Sodium hydroxide (alkali flakes, purity greater than 99%), sodium silicate (27.3 wt.% SiO 2 , 8.54 wt.% Na 2 O, and 64.16 wt.% H 2 O), and tap water were used to prepare the alkali activator. the adhesion of the geopolymer to the cement interface. The findings of this paper will aid in further optimizing the mix ratio of MK-GGBS-based geopolymer repair mortar as well as understanding its comprehensive performance as a repair material.

Raw Materials
MK, GGBS, and ordinary Portland cement (OPC) used in this study are all commercially available materials. The chemical composition of the precursor was determined by X-ray fluorescence spectrometer (XRF), as shown in Table 1. MK has the same SiO2 content as GGBS, but MK has more Al2O3 and GGBS has more CaO. The microstructure of MK and GGBS is shown in Figure 1. MK is a flake and GGBS is an angular particle. Figure 2a and Table 2 show the particle size of the precursors, with the mean particle size (D50) of MK and GGBS being 4.5 μm and 13.17 μm, respectively. Figure 2b shows the XRD pattern of the precursor. The main crystalline phases of MK are corundum, pseudorutile, and zircon, while the main crystalline phases of GGBS are quartz and calcium magnesium phosphate. International Standards Organization (ISO) sand is used as fine aggregate, and its physical properties are shown in Table 3. Sodium hydroxide (alkali flakes, purity greater than 99%), sodium silicate (27.3 wt.% SiO2, 8.54 wt.% Na2O, and 64.16 wt.% H2O), and tap water were used to prepare the alkali activator.

Experimental Design by RSM
The Box Behnken design (BBD) and Central Composite design (CCD) methods are commonly used in RSM. BBD can reduce the number of experiments with the same factors and levels, and CCD can better fit the surface by taking extreme points; however, taking extreme values leads to poor test results because the factor levels are outside the normal range, so the BBD method was used to ensure test accuracy. GGBS content (factor ), Na2O/binder ratio (factor ), SiO2/Na2O molar ratio (factor ), and water/binder ratio (factor ) were selected as influencing factors, with three levels for each factor. The value was determined by the preliminary experiment, as shown in Table 4. In order to utilize the advantages of fast setting and high early strength of the MK-GGBS-based geopolymer in the field of rapid repair, the 1 d compressive strength ( ), 1 d flexural strength ( ), and 1 d bond strength ) were selected as the evaluation indices in combination with the requirements of the Chinese standard for repair mortars (JC/T 2381-2016) and the Chinese technical specifications for pavements (JTJ0731-2001 and JTG D40-2011). The specific test scheme is shown in Table 5.

Experimental Design by RSM
The Box Behnken design (BBD) and Central Composite design (CCD) methods are commonly used in RSM. BBD can reduce the number of experiments with the same factors and levels, and CCD can better fit the surface by taking extreme points; however, taking extreme values leads to poor test results because the factor levels are outside the normal range, so the BBD method was used to ensure test accuracy. GGBS content (factor A), Na 2 O/binder ratio (factor B), SiO 2 /Na 2 O molar ratio (factor C), and water/binder ratio (factor D) were selected as influencing factors, with three levels for each factor. The value was determined by the preliminary experiment, as shown in Table 4. In order to utilize the advantages of fast setting and high early strength of the MK-GGBS-based geopolymer in the field of rapid repair, the 1 d compressive strength (y 1 ), 1 d flexural strength (y 2 ), and 1 d bond strength (y 3 ) were selected as the evaluation indices in combination with the requirements of the Chinese standard for repair mortars (JC/T 2381-2016) and the Chinese technical specifications for pavements (JTJ0731-2001 and JTG D40-2011). The specific test scheme is shown in Table 5.

Sample Preparation
Geopolymer mortar was prepared according to Table 5. The alkali activator solution was first prepared by mixing sodium hydroxide with water and stirring well to obtain a sodium hydroxide solution, then the water glass was added to the sodium hydroxide solution and stirred well and cooled for 24 h in a laboratory environment. To make the mortar, MK, GGBS and sand were mixed together for 2 min at low speed to create a homogeneous mixture of solids. Then, alkali activator solution was added and mixed at low speed for 2 min, then at high speed for 2 min. The fresh mortar is injected into the mold in two stages, with each vibration lasting 60 strokes. After vibration, it is be covered with cling film and cured in the laboratory environment (temperature: 25 • C, humidity: 60%) until testing.

Test Methods
The setting time test was based on the Chinese national standard GB/T 50080 test setting time with a penetration resistance meter. The test of compressive and flexural strength was based on the Chinese national standard GB/T 17671-2021. For the flexural strength test, mortar samples of 40 mm × 40 mm × 160 mm are used. A pressure testing machine (TSY-2000 constant loading pressure testing machine) was used for loading, and the loading rate was 50 N/s. Three samples were prepared for each group, and the test results were averaged. The compressive strength of the broken prisms is tested. The compressive surface is the two sides of the test body when it is formed, and the area is 40 mm by 40 mm. A pressure testing machine (TSY-2000 constant loading pressure testing machine) was used for loading, with a loading rate of 2.4 KN/s. Six samples were prepared for each group, and the test results were averaged. The bond strength test is shown in Figure 3. Two methods were used to test the bond strength. The slant shear test was used to evaluate the strength value [31], and the flexural bending strength test was used to evaluate the adhesion effect and failure mode of the interface. The cement mortar was first created as a substrate by filling one side of the 40 mm × 40 mm × 160 mm mold with extruded polystyrene foam and the cement mortar (sand:cement:water = 3:1:0.5) was poured on the other side, and then demolded and conditioned in a laboratory environment for 28 days. The cement substrate was then placed on one side of the 40 mm × 40 mm × 160 mm mold, and the bonded surface had been sandpapered smooth in advance to eliminate the effect of roughness [8]. In the other side a geopolymer mortar was poured, and then it was demolded and cured in a laboratory environment until tested. After curing in the laboratory environment, a pressure testing machine (TSY-2000 constant loading pressure testing machine) was used for loading according to the loading method shown in Figure 3, and the loading rate was 50 N/s. Equations (2) and (3) were used to calculate the slant shear strength and flexural bending strength. A set of three specimens were averaged to determine the bond strength value.
the loading rate was 50 N/s. Three samples were prepared for each group, and the test results were averaged. The compressive strength of the broken prisms is tested. The compressive surface is the two sides of the test body when it is formed, and the area is 40 mm by 40 mm. A pressure testing machine (TSY-2000 constant loading pressure testing machine) was used for loading, with a loading rate of 2.4 KN/s. Six samples were prepared for each group, and the test results were averaged.
The bond strength test is shown in Figure 3. Two methods were used to test the bond strength. The slant shear test was used to evaluate the strength value [31], and the flexural bending strength test was used to evaluate the adhesion effect and failure mode of the interface. The cement mortar was first created as a substrate by filling one side of the 40 × 40 mm × 160 mm mold with extruded polystyrene foam and the cement mortar (sand : cement : water = 3 : 1 : 0.5) was poured on the other side, and then demolded and conditioned in a laboratory environment for 28 days. The cement substrate was then placed on one side of the 40 mm × 40 mm × 160 mm mold, and the bonded surface had been sandpapered smooth in advance to eliminate the effect of roughness [8]. In the other side a geopolymer mortar was poured, and then it was demolded and cured in a laboratory environment until tested. After curing in the laboratory environment, a pressure testing machine (TSY-2000 constant loading pressure testing machine) was used for loading according to the loading method shown in Figure 3, and the loading rate was 50 N/s. Equations where is the slant shear strength (MPa), is the flexural bending strength (MPa), and F is the loading force when the sample fails (N).
The water absorption test was based on the Chinese standard JG/T 2381-2016. A 40 mm × 40 mm × 80 mm geopolymer mortar specimen was prepared, of which a 40 mm × 40 mm surface was the test surface. After curing for 28 d in the laboratory environment, the specimen was put into a 70 °C blast drying oven and dried to a constant weight. After cooling to room temperature, five surfaces except the test surface were coated with sealing materials, and the mass of the specimen was weighed. The specimen was vertically placed on a 25 g/L~30 g/L saturated polyurethane sponge filled with water, face down. At (2) where f s is the slant shear strength (MPa), f f is the flexural bending strength (MPa), and F is the loading force when the sample fails (N). The water absorption test was based on the Chinese standard JG/T 2381-2016. A 40 mm × 40 mm × 80 mm geopolymer mortar specimen was prepared, of which a 40 mm × 40 mm surface was the test surface. After curing for 28 d in the laboratory environment, the specimen was put into a 70 • C blast drying oven and dried to a constant weight. After cooling to room temperature, five surfaces except the test surface were coated with sealing materials, and the mass m a of the specimen was weighed. The specimen was vertically placed on a 25 g/L~30 g/L saturated polyurethane sponge filled with water, face down. At 6 h and 72 h, the surface of the specimen was wiped dry to measure the mass (m b ). The water absorption of the mortar was calculated according to Equation (4): where W ab is the amount of water absorbed in 6 h or 72 h (kg/m 2 ), m a is the mass of the specimen before immersion (g), and m b is the mass of the specimen after immersion (g). The shrinkage test of the mortar was based on the Chinese standard JC/T 603. When the specimen's compressive strength reached (10 ± 2) MPa, the initial length L 0 of the test piece was measured within 30 min of its release. The length of the specimen was measured at 1 d-7 d, 14 d, and 28 d, denoted as L t . The shrinkage rate of the mortar was calculated according to Equation (5): where S t is the shrinkage rate at time t (%), t = 1-7 d, 14 d, and 28 d, L 0 is the initial measurement reading (mm), L t is the measured reading at time t (mm), and 250 is the effective length of the specimen (mm). The efflorescence of materials was assessed by visual observation [32]. The mortar test of 40 × 40 × 80 mm was placed vertically in water with a depth of 40 mm along the length direction of 80 mm after curing for 28 d, as shown in Figure 4. After curing for 28 d in the laboratory environment, the efflorescence degree of the samples was observed visually.
water absorption of the mortar was calculated according to Equation (4): where is the amount of water absorbed in 6 h or 72 h (kg/m 2 ), is the mass specimen before immersion (g), and is the mass of the specimen after immersio The shrinkage test of the mortar was based on the Chinese standard JC/T 603. W the specimen's compressive strength reached (10 ± 2) MPa, the initial length of th piece was measured within 30 min of its release. The length of the specimen was mea at 1 d-7 d, 14 d, and 28 d, denoted as . The shrinkage rate of the mortar was calcu according to Equation (5): where is the shrinkage rate at time t (%), t = 1-7 d, 14 d, and 28 d, is the i measurement reading (mm), is the measured reading at time t (mm), and 250 effective length of the specimen (mm).
The efflorescence of materials was assessed by visual observation [32]. The m test of 40 × 40 × 80 mm was placed vertically in water with a depth of 40 mm alon length direction of 80 mm after curing for 28 d, as shown in Figure 4. After curing d in the laboratory environment, the efflorescence degree of the samples was obs visually. BSE and EDS observed the interface between the geopolymer-repairing sampl matrix, as shown in Figure 5. First, the cement sample (cement: water = 1 : 0.5) wa pared, cured for 28 d in the laboratory environment, and then poured into the geopol slurry. After curing for 24 h, isopropyl alcohol was used to terminate the hydration obtained samples [14]. The sample was dried and then inlaid with epoxy resin unde uum. An automatic polisher was used to sand and polish the sample until a smooth face was obtained. BSE and EDS observed the interface between the geopolymer-repairing sample and matrix, as shown in Figure 5. First, the cement sample (cement:water = 1:0.5) was prepared, cured for 28 d in the laboratory environment, and then poured into the geopolymer slurry. After curing for 24 h, isopropyl alcohol was used to terminate the hydration of the obtained samples [14]. The sample was dried and then inlaid with epoxy resin under vacuum. An automatic polisher was used to sand and polish the sample until a smooth surface was obtained.

RSM Results and Analysis
According to the 29 combinations in Table 5, 1 d compressive strength, 1 d flexural strength, and 1 d bond strength of geopolymer mortar were tested, and the test results are shown in Table 6.

RSM Results and Analysis
According to the 29 combinations in Table 5, 1 d compressive strength, 1 d flexural strength, and 1 d bond strength of geopolymer mortar were tested, and the test results are shown in Table 6. Design-Expert software was used to analyze the applicability of the mathematical model obtained from the test data, and the analysis of variance (ANOVA) results of the model were obtained, as shown in Table 7. In Table 7, the interaction of factors A and B are represented in the table, and the symbols in the table represent factors and the interaction between factors.  Table 7 shows that the p value for the "model" terms for 1 d compressive strength, 1 d flexural strength, and 1 d bond strength are less than 0.0001, while the p value for "Lack of Fit" < 0.05. p values are commonly used to validate the significance of the regression coefficient, and models with p < 0.05 are generally considered significant, while models with p > 0.05 are considered insignificant. This indicates that the three regression models y 1 , y 2 , and y 3 are significant, while their misfit terms are insignificant. In addition, the R 2 of the three models are 0.9849, 0.9844, and 0.9758, respectively, and the adjusted R 2 are 0.9697, 0.9688, and 0.9515, respectively, which are all greater than 0.95, indicating that these models can effectively explain the changes in response values and are suitable for predictive analysis, and the analysis was conducted at the 5% level of significance. Based on the results of the experiment, the prediction functions of y 1 , y 2 , and y 3 were obtained by ANOVA as shown in Equations (6)-(8): According to the "p-value" in Table 7, it is clear that for 1 d compressive strength, factors A, B, and D have a highly significant effect (p < 0.0001), and factor C has a nonsignificant effect (p > 0.05). Meanwhile, there is a significant interaction between factors A × C, factors A × D, and factors C × D. Based on the magnitude of the "F-value", it can be seen that the significant effects of each factor on 1 d compressive strength is as follows:  [33]. Figure 8 shows that when the GGBS content is fixed, with the increase in the SiO 2 /Na 2 O molar ratio, the 1 d compressive strength of geopolymer first increases and then decreases, reaching the maximum value between 1.15 and 1.25, which is close to the results of many studies [4,7]. In fact, the dissolution of silicate monomer in the precursor is more difficult than that of aluminate monomer. Therefore, the introduction of sodium silicate can provide soluble silicate to accelerate the geopolymer reaction [22]. However, when the SiO 2 /Na 2 O molar ratio is too high, the alkali concentration will be reduced accordingly, and the generated silicate monomer will also be adsorbed on the surface of solid particles, hindering the reaction. Figure 7 shows that when GGBS content is fixed, the strength of geopolymer increases slightly and then decreases, reaching the maximum value between 0.42 and 0.44, which is related to the low flowability of geopolymer when the ratio of MK is high. Appropriately increasing the water/binder ratio can improve its fluidity, and expand the spacing between particles to promote dissolution and make the structure denser. Further increase in water will result in increased porosity and decreased structure strength. Figure 8 shows that with the increase in the SiO 2 /Na 2 O molar ratio and the water/binder ratio, the 1 d compressive strength first increases and then decreases. When the SiO 2 /Na 2 O molar ratio is 1.15~1.25 and the water/binder ratio is 0.4~0.44, the maximum values can be obtained. When the SiO 2 /Na 2 O molar ratio is 1.4 and the water/binder ratio is 0.5, the compressive strength is only 17 MPa, which is because the alkalinity of the solution is low and the precursors cannot be fully excited [16].
the water/binder ratio can improve its fluidity, and expand the spacing between particles to promote dissolution and make the structure denser. Further increase in water will result in increased porosity and decreased structure strength. Figure 8 shows that with the increase in the SiO2/Na2O molar ratio and the water/binder ratio, the 1 d compressive strength first increases and then decreases. When the SiO2/Na2O molar ratio is 1.15~1.25 and the water/binder ratio is 0.4~0.44, the maximum values can be obtained. When the SiO2/Na2O molar ratio is 1.4 and the water/binder ratio is 0.5, the compressive strength is only 17 MPa, which is because the alkalinity of the solution is low and the precursors cannot be fully excited [16].

Flexural Strength of 1 d
According to the "p-value" value in Table 7, factor has a significant effect on 1 d flexural strength when compared with 1 d compressive strength (p = 0.0133), and there is also an interaction between factor × . Based on the magnitude of the "F-value," it can be seen that the significance of each factor on 1 d flexural strength is as follows:  Figure 11 shows that with the increase in the Na2O/binder ratio, 1 d flexural strength first increases and then decreases, and the maximum value is reached when the Na2O/binder ratio is 10~10.5%, which shows a consistent rule under different GGBS con-

Flexural Strength of 1 d
According to the "p-value" value in Table 7, factor has a significant effect on 1 d flexural strength when compared with 1 d compressive strength (p = 0.0133), and there is also an interaction between factor × . Based on the magnitude of the "F-value," it can be seen that the significance of each factor on 1 d flexural strength is as follows:  Figure 11 shows that with the increase in the Na2O/binder ratio, 1 d flexural strength first increases and then decreases, and the maximum value is reached when the Na2O/binder ratio is 10~10.5%, which shows a consistent rule under different GGBS con-

Flexural Strength of 1 d
According to the "p-value" value in Table 7, factor C has a significant effect on 1 d flexural strength when compared with 1 d compressive strength (p = 0.0133), and there is also an interaction between factor A × B. Based on the magnitude of the "F-value", it can be seen that the significance of each factor on 1 d flexural strength is as follows:  Figure 11 shows that with the increase in the Na 2 O/binder ratio, 1 d flexural strength first increases and then decreases, and the maximum value is reached when the Na 2 O/binder ratio is 10~10.5%, which shows a consistent rule under different GGBS contents. An appropriate Na 2 O/binder ratio can provide a suitable alkaline environment for the dissolution of solid precursors. If the Na 2 O/binder ratio is too low, the efficiency of the solid dissolution of the silicaluminate monomer is low; if the ratio is too high, it will cause the dissolution of the silicaluminate oligomer and the reduction in free water, thus reducing the reaction rate [34]. The rule in Figures 10-12 are consistent with the results of 1 d compressive strength. Especially in Figure 14, when the GGBS content is 60%, the decline in the flexural strength with the water/binders ratio is significantly slower than that when the GGBS content is 40%. Obviously, more GGBS incorporation effectively improves the impact of the increase in the water/binder ratio on 1 d flexural strength.

Bond Strength of 1 d
According to the "p-value" in Table 7, the 1 d bond strength and 1 d flexural strength are consistent in terms of the significance of the single factors. In the interaction between factors, there are significant interactions between factors × , factors × , and factors × . The significance of each factor of 1 d bond strength is as follows:  Figure 13 shows that as the Na2O/binder ratio increases, the 1 d bond strength increases first and then decreases, reaching its maximum value when the Na2O/binder ratio is between 10% and 10.5%. Different from 1 d flexural strength, when 1 d bond strength exceeds the peak value, the bond strength declines more slowly as the Na2O/binder ratio continues to increase, which may be due to the reaction of part of the alkali solution with the cement matrix [35]. This indicates that a high Na2O/binder ratio is beneficial for bond strength. The results of Figures 14 and 15 are consistent with those of compressive and flexural resistance. In particular, it was found that, compared with the 1 d compressive strength and 1 d flexural strength, the 1 d bond strength decreased more slowly in the SiO2/Na2O molar ratio from 1.2 to 1.0, which is consistent with Figure 15. Lower SiO2/Na2O molar ratios corresponded to higher Na2O content. This further illustrates the benefits of higher alkalinity for bonding.

Bond Strength of 1 d
According to the "p-value" in Table 7, the 1 d bond strength and 1 d flexural strength are consistent in terms of the significance of the single factors. In the interaction between factors, there are significant interactions between factors A × B, factors A × C, and factors C × D. The significance of each factor of 1 d bond strength is as follows:  Figure 13 shows that as the Na 2 O/binder ratio increases, the 1 d bond strength increases first and then decreases, reaching its maximum value when the Na 2 O/binder ratio is between 10% and 10.5%. Different from 1 d flexural strength, when 1 d bond strength exceeds the peak value, the bond strength declines more slowly as the Na 2 O/binder ratio continues to increase, which may be due to the reaction of part of the alkali solution with the cement matrix [35]. This indicates that a high Na 2 O/binder ratio is beneficial for bond strength. The results of Figures 14 and 15 are consistent with those of compressive and flexural resistance. In particular, it was found that, compared with the 1 d compressive strength and 1 d flexural strength, the 1 d bond strength decreased more slowly in the SiO 2 /Na 2 O molar ratio from 1.2 to 1.0, which is consistent with Figure 15. Lower SiO 2 /Na 2 O molar ratios corresponded to higher Na 2 O content. This further illustrates the benefits of higher alkalinity for bonding.
strength. The results of Figures 14 and 15 are consistent with those of compressive and flexural resistance. In particular, it was found that, compared with the 1 d compressive strength and 1 d flexural strength, the 1 d bond strength decreased more slowly in the SiO2/Na2O molar ratio from 1.2 to 1.0, which is consistent with Figure 15. Lower SiO2/Na2O molar ratios corresponded to higher Na2O content. This further illustrates the benefits of higher alkalinity for bonding.

RSM Solving and Verification
In the Design-Expert software, the target of 1 d compressive strength, 1 d flexural

RSM Solving and Verification
In the Design-Expert software, the target of 1 d compressive strength, 1 d flexural

RSM Solving and Verification
In the Design-Expert software, the target of 1 d compressive strength, 1 d flexural strength, and 1 d bond strength was set as the maximum, and the levels of each factor were obtained as follows: A = 60%, B = 10.2%, C = 1.19, and D = 0.41, and the ratio was recorded as Mix RSM. In order to verify the prediction model of RSM, tests were carried out again for Mix RSM, three times for each group, and the average value was taken. The test results are shown in Figure 16. The results show that the relative error between the predicted values of the model and the experimental results is less than 3%. The results predicted by the model can reflect the real-life test situation.

Performance Test of Geopolymer Repairing Mortar
The results of RSM show that GGBS content is the main factor affecting t of the geopolymer repair mortar. This is related to the change in gel comp geopolymer when MK and GGBS are mixed in a certain proportion [36], and ingly, its performance as a repair material will also change. In order to exp properties of Mix RSM repair mortar and the influence of GGBS content, fo studies, the Na2O/binder ratio, SiO2/Na2O molar ratio, and water/binder rat mended values, and the GGBS content should be set at 0, 60%, and 100% (lab Mix RSM, and Mix GGBS, respectively). Figure 17 records the test results of the setting time. Compared with initial setting time of Mix RSM and Mix GGBS is reduced by 67% and 75%, setting time is reduced by 75% and 82%, respectively. Obviously, the inc GGBS is beneficial for rapid coagulation. This is due to the higher bond ener O and Al-O bonds, and it takes longer to break down. Conversely, the bond O is lower and it can react with [SiO4] 4− in the alkali activator solution mo form C-S-H gel and encourage coagulation [33,35,37]. The setting time of M Mix GGBS is similar, indicating that GGBS with a 60% replacement rate ca

Performance Test of Geopolymer Repairing Mortar
The results of RSM show that GGBS content is the main factor affecting the properties of the geopolymer repair mortar. This is related to the change in gel composition of the geopolymer when MK and GGBS are mixed in a certain proportion [36], and correspondingly, its performance as a repair material will also change. In order to explore the other properties of Mix RSM repair mortar and the influence of GGBS content, for subsequent studies, the Na 2 O/binder ratio, SiO 2 /Na 2 O molar ratio, and water/binder ratio are recommended values, and the GGBS content should be set at 0, 60%, and 100% (labeled Mix MK, Mix RSM, and Mix GGBS, respectively). Figure 17 records the test results of the setting time. Compared with Mix MK, the initial setting time of Mix RSM and Mix GGBS is reduced by 67% and 75%, and the final setting time is reduced by 75% and 82%, respectively. Obviously, the incorporation of GGBS is beneficial for rapid coagulation. This is due to the higher bond energies of the Si-O and Al-O bonds, and it takes longer to break down. Conversely, the bond energy of Ca-O is lower and it can react with [SiO 4 ] 4− in the alkali activator solution more quickly to form C-S-H gel and encourage coagulation [33,35,37]. The setting time of Mix RSM and Mix GGBS is similar, indicating that GGBS with a 60% replacement rate can achieve the same setting time as the GGBS-based geopolymer mortar. Meanwhile, Mix RSM and Mix GGBS meet the requirements of JC/T 2381-2016: initial setting time ≤ 30 min; final setting time ≤ 50 min.

Setting Time
Mix GGBS is similar, indicating that GGBS with a 60% replacem same setting time as the GGBS-based geopolymer mortar. Meanw GGBS meet the requirements of JC/T 2381-2016: initial setting tim time ≤ 50 min.   [14,38], but due to the gel's rapid generation, the gel will wrap around the reactant particles. As a result, the subsequent strength development was stymied, and the strength of Mix GGBS almost did not develop from 7 d to 28 d, while the strength of Mix MK exceeded the strength of Mix GGBS in this case. The intensity of the Mix RSM was high (18.65 MPa at 6 h) in the early stage of the reaction due to the presence of more GGBS, and continued to increase in the late stage due to the presence of MK. Mix RSM has the highest strength from 1 d to 28 d because the gels produced by MK and GGBS can be combined to make the structure more dense. The bond strength of the geopolymer mortar test results is depicted in Figure 18b. The bond strength followed a similar pattern to the compressive strength, with the exception that at 1 d, the bond strength of Mix MK was already higher than that of Mix GGBS. Table 8 records the compressive and bond strengths specified in JC/T 2381-2016. Therefore, the compressive and bond strengths of Mix RSM and Mix GGBS meet the requirements. Figure 19 depicts the bond strength specimens breaking. The specimens all break on the geopolymer side at 6 h, but Mix RSM has less geopolymer adhering to the cement side than Mix MK and Mix GGBS, which is consistent with the test results of bond strength. At 28 d, the specimens all break on the cement matrix side, indicating that the geopolymer's adhesion strength to the cement matrix exceeds the cement matrix's strength. Table 9 records the bond strength values of the repair mortar tested by some scholars [15,31,[38][39][40][41][42], and the method adopted is consistent with this study. Geopolymer repair mortar has a higher bonding strength than some conventional and modified repair materials. Although magnesium phosphate cement (MPC) repair mortar has a strength of 4.1 MPa in 1 d, its preparation via an acid-base reaction is costly, and its compressive strength in contact with water is greatly reduced [43], severely limiting its application. In addition, compared with the bond strength of other geopolymers listed in Table 9, Mix RSM has higher bond strengths of 1 d and 28 d. Although different raw materials and preparation processes may lead to bias in the results, it also indicates that the RSM method can optimize the performance of geopolymer repair mortar to a certain extent. cement (MPC) repair mortar has a strength of 4.1 MPa in 1 d, its preparation via an acidbase reaction is costly, and its compressive strength in contact with water is greatly reduced [43], severely limiting its application. In addition, compared with the bond strength of other geopolymers listed in Table 9, Mix RSM has higher bond strengths of 1 d and 28 d. Although different raw materials and preparation processes may lead to bias in the results, it also indicates that the RSM method can optimize the performance of geopolymer repair mortar to a certain extent.      The results of the shrinkage test are shown in Figure 20. In the first few days, the

Shrinkage
The results of the shrinkage test are shown in Figure 20. In the first few days, the specimen would first expand, at which time the expansion of Mix MK was larger and the expansion value of Mix RSM was close to that of Mix GGBS. This is due to the geopolymer's chemical swelling. Swelling in MK-based geopolymers may be caused by the continuous movement of water from the macropores into the mesopores, as well as salt precipitation and the formation of the crystalline zeolite phase, both of which can cause swelling [44][45][46]. Although shrinkage is the dominant phenomenon in GGBS-based geopolymers, there is also volume expansion due to crystalline phase swelling [47]. The swelling occurs early in the reaction, followed by shrinkage.

Water Absorption and Efflorescence
Water absorption reflects the water resistance of the geopolymer mortar and erence for the repair of structures exposed to humid environments. Especially, geopolymer is prone to efflorescence in humid environments, there is a certain r ship between water absorption and efflorescence resistance. Figure 21 shows the ymer's water absorption over the course of 6 h and 72 h. According to the findin MK has a very high water absorption of 5.69 kg/m 2 and 9.35 kg/m 2 at 6 h and 72 h is much higher than the 1.  Figure 22 shows the result of the visual efflores geopolymer mortar. Mix MK exhibits the most severe visual weathering and a sig amount of crystallization, followed by Mix GGBS. In contrast, Mix RSM only ex white layer of lye bleed on the surface without any discernible weathering crystal It is in line with the findings regarding water absorption and indicates that the g mer's water and weathering resistance is further improved when the ratio of MK t is suitable.

Water Absorption and Efflorescence
Water absorption reflects the water resistance of the geopolymer mortar and is a reference for the repair of structures exposed to humid environments. Especially, because geopolymer is prone to efflorescence in humid environments, there is a certain relationship between water absorption and efflorescence resistance. Figure 21 shows the geopolymer's water absorption over the course of 6 h and 72 h. According to the findings, Mix MK has a very high water absorption of 5.69 kg/m 2 and 9.35 kg/m 2 at 6 h and 72 h, which is much higher than the 1.2 kg/m 2 and 2.0 kg/m 2 recommended by JC/T 2381-2016. In contrast, water absorption is reduced in Mix RSM and Mix GGBS due to the denser structural makeup; for instance, the values of water absorption are respectively 0.64 kg/m 2 and 0.69 kg/m 2 at 6 h, while they are respectively 1.21 kg/m 2 and 1.43 kg/m 2 at 72 h. It should be pointed out that the values of water absorption of both Mix RSM and Mix GGBS meet the requirements of the standard. Figure 22 shows the result of the visual efflorescence of geopolymer mortar. Mix MK exhibits the most severe visual weathering and a significant amount of crystallization, followed by Mix GGBS. In contrast, Mix RSM only exhibits a white layer of lye bleed on the surface without any discernible weathering crystallization. It is in line with the findings regarding water absorption and indicates that the geopolymer's water and weathering resistance is further improved when the ratio of MK to GGBS is suitable. amount of crystallization, followed by Mix GGBS. In contrast, Mix R white layer of lye bleed on the surface without any discernible weathe It is in line with the findings regarding water absorption and indicate mer's water and weathering resistance is further improved when the r is suitable.   Figure 23 depicts the results of the BSE testing. The Mix RSM a were denser and contained more unreacted particles than the Mix MK to the fact that the C-(A)-S-H gel is adsorbed on the surface of the reac filling the structure, preventing further development of the reaction [1 fewer unreacted large particles and more gel than Mix GGBS, which higher strength of Mix RSM. In addition, it can be seen that the in groups and the cement is well bonded. This further illustrates the ad ymers as repair materials. The chemical elements of the interface are The Ca/Si of Mix MK, Mix GGBS, and Mix RSM were 0.81, 1.04, an Because the alkali activator can react with Ca(OH)2 in cement to prod H gels [35,49,50]. The Ca/Si of Mix RSM is the lowest, which means t S-H gel and less Ca(OH)2 on the interface of Mix RSM, which makes  Figure 23 depicts the results of the BSE testing. The Mix RSM and Mix GGBS gels were denser and contained more unreacted particles than the Mix MK gels. This is related to the fact that the C-(A)-S-H gel is adsorbed on the surface of the reactant particles while filling the structure, preventing further development of the reaction [16,48]. Mix RSM has fewer unreacted large particles and more gel than Mix GGBS, which is the reason for the higher strength of Mix RSM. In addition, it can be seen that the interface between all groups and the cement is well bonded. This further illustrates the advantages of geopolymers as repair materials. The chemical elements of the interface are shown in Figure 24. The Ca/Si of Mix MK, Mix GGBS, and Mix RSM were 0.81, 1.04, and 0.53, respectively. Because the alkali activator can react with Ca(OH) 2 in cement to produce low-Ca/Si C-S-H gels [35,49,50]. The Ca/Si of Mix RSM is the lowest, which means that there is more C-S-H gel and less Ca(OH) 2 on the interface of Mix RSM, which makes the transition zone of the interface more dense. This is also the reason for the higher bond strength of Mix RSM.

BSE and EDS
ymers as repair materials. The chemical elements of the interface are shown in Figure 24. The Ca/Si of Mix MK, Mix GGBS, and Mix RSM were 0.81, 1.04, and 0.53, respectively. Because the alkali activator can react with Ca(OH)2 in cement to produce low-Ca/Si C-S-H gels [35,49,50]. The Ca/Si of Mix RSM is the lowest, which means that there is more C-S-H gel and less Ca(OH)2 on the interface of Mix RSM, which makes the transition zone of the interface more dense. This is also the reason for the higher bond strength of Mix RSM.

Conclusions
In order to optimize the proportion of MK-GGBS-based geopolymer repair mortar, the RSM method was used to investigate the effects of GGBS content, Na2O/binder ratio, SiO2/Na2O molar ratio, and water/binder ratio, and their interactions on 1 d compressive strength, 1 d flexural strength, and 1 d bond strength. Setting time, long-term mechanical properties, shrinkage, water absorption, and efflorescence potential of the optimized geopolymer repair were discussed. The main conclusions are as follows:


Based on RSM, the prediction models of 1 d compressive strength, 1 d flexural strength, and 1 d bond strength of MK-GGBS-based geopolymer mortar were established at the significant level of 5%. ANOVA analysis results showed that GGBS content, water/binder ratio, and Na2O/binder ratio had significant effects on each response, and SiO2/Na2O molar ratio had significant effects on 1 d flexural strength and

Conclusions
In order to optimize the proportion of MK-GGBS-based geopolymer repair mortar, the RSM method was used to investigate the effects of GGBS content, Na 2 O/binder ratio, SiO 2 /Na 2 O molar ratio, and water/binder ratio, and their interactions on 1 d compressive strength, 1 d flexural strength, and 1 d bond strength. Setting time, long-term mechanical properties, shrinkage, water absorption, and efflorescence potential of the optimized geopolymer repair were discussed. The main conclusions are as follows: • Based on RSM, the prediction models of 1 d compressive strength, 1 d flexural strength, and 1 d bond strength of MK-GGBS-based geopolymer mortar were established at the significant level of 5%. ANOVA analysis results showed that GGBS content, water/binder ratio, and Na 2 O/binder ratio had significant effects on each response, and SiO 2 /Na 2 O molar ratio had significant effects on 1 d flexural strength and 1 d bond strength; the effect on 1 d compressive strength was not significant.

•
The RSM analysis results showed that the 1 d compressive strength, 1 d flexural strength, and 1 d bond strength were all proportional to the GGBS content, increasing and then decreasing with the increase in Na 2 O/binder ratio, SiO 2 /Na 2 O molar ratio, and water/binder ratio, with maximum values at 10%~10.5%, 1.15~1.25, and 0.42~0.44, respectively. When the SiO 2 /Na 2 O molar ratio was 1.4 and the water/binder ratio was 0.5, the alkalinity of the solution was low, the precursor could not be fully excited, and the 1 d compressive strength was only 17 MPa. When the water/binder ratio increased from the optimal range to 0.5, the decline rate of 1 d flexural strength decreased significantly with the increase in GGBS. When the Na 2 O/binder ratio increases from the optimal range to 11% and the SiO 2 /Na 2 O molar ratio from 1.2 to 1.0, the bond strength declines slowly, and high alkalinity is beneficial to the bond strength. The results of BSE showed that the geopolymer was tightly bound to the matrix. EDS results showed that compared with the geopolymer mortar based on MK and GGBS, Mix RSM had lower Ca/Si at the interface, more C-S-H gel, and less Ca(OH) 2 at the interface, and the interface was denser.
Research has shown that RSM enables the optimization of the design of geopolymer ratios, but the response of the optimum design is determined by the purpose of rapid repair. In practice, repair mortars must meet a number of requirements, including self-compaction, corrosion resistance, and high abrasion resistance. Proportional optimization with the help of RSM is also required for the performance of geopolymer repair mortars in these application scenarios.